### Numerical assessment of failure

### mechanisms in fibre metal laminates

Frank Hashagen and Rene de BorstDelft University of Technology, Koiter Institute Delft, P.O. Box 5048, 2600 GA Delft, The Netherlands, email: F.Hashagen@CT.tudelft.nl

In this contribution numerical models are discussed for describing failure mechanisms in fibre metal laminates. Fibre metal laminates form a new class of materials which are considered for a possible application to the fuselage of future aircraft generations. The intensive experimental analyses of these materials are focused on the assessment of their residual strength and on the assessment of new design methods. To support the experimental analyses numerical models are used to describe cracking and delamination in fibre metal laminates. A special continuum element and a corresponding interface element are introduced. Furthermore, loading functions are applied which account for cracking and delamination. Subsequently, results are discussed which are obtained from numerical analyses of the residual strength of plates made of GLARETM . Finally, the splicing technique as a new design method is assessed by a comparison between numerical and experimental results.

*Key words: *fibre metal laminates, solid-like shell, interface elements, crack growth, residual strength,
delamination, splices

### 1

### Description of fibre metal laminates

Fibre metal laminates are bonded arrangements of thin aluminium layers and prepreg layers that are reinforced either by glass fibres or by aramid fibres, Figure 1. They have been pioneered at the Faculty of Aerospace Engineering of Delft University of Technology. Due to its fatigue resistance and fracture characteristics the fibre metal laminate GLARE''' shows a high potential to serve as skin material for the fuselage of a new super large aircraft, the AIRBUS A3XX. However, before fibre metal laminates can be applied intensive testing is necessary to evaluate the characteristics of the material and to derive the corresponding material parameters. Furthermore, fibre metallami-nates offer the possibility to apply new design methods which make use of their layered structure. Commonly, the fuselage of an aircraft is composed of a number of aluminium sheets. Their width determines the number of joints that add to the structural weight of the fuselage. By applying the so-called splicing technique the width of the sheets can be increased which subsequently reduces the weight of the structure.

Due to the economical interest in fibre metal laminates and their possible application to the fuselage of the A3XX the experimental research is carried out under strict time and cost constraints. Since testing is time consuming and expensive numerical strategies are necessary to enhance the development of fibre metal laminates. Furthermore, the complex structure of the material requires a

theoretical verification of the results that are obtained applying design methods which are derived for homogeneous materials. Especially the residual strength (strength of the material in the pres-ence of cracks) and the impact of the splicing technique are major points of concern [10].

For the derivation of the numerical models several aspects must be taken into consideration. First, a continuum element is derived. It is imperative that the continuum element describes fibre metal laminates in a three-dimensional state. This goal is achieved with a solid-like shell element. Sec-ondly, interface elements are applied at the locations where cracking or delamination is expected to occur. They are consistent to the formulation of the continuum elements. Thirdly, the failure mecha-nisms cracking and delamination must be accounted for. Here, cracking determines the residual strength of the fibre metal laminates and delamination has a significant impact on spliced struc-tures. Both mechanisms are described by applying interface elements and introducing a loading function which bounds all states of the stress in the interface elements.

In the following the continuum element and the interface element are introduced briefly. Subse-quently, the interface crack model is described and applied for a residual strength analysis of a cen-tre cracked plate made of the fibre metal laminate GLARETM. Finally, the impact of splices is studied with spliced tension specimen made of GLARFM .

**Aluminium **

*Fig. *1. *Schematic sketch of the lay-up of fibre metal laminates. *

### 2

### Applied finite elements

*2.1*

*Solid-like shell element*

Typically, structures made of fibre metal laminates are very thin. For these applications shell elements are widely used in finite element calculations. However, the description of delamination in a three-dimensional manner is difficult with shell elements. The reason lies in the separation of the different layers when delamination occurs. This is often accompanied by strains and stresses in the thickness direction which are not incorporated in most shell theories. Alternatively, solid

elements can be applied. However, these elements tend to lock in thin applications. Hence, a new class of elements, so-called solid-like shell elements [4, 12], is applied to describe fibre metallami-nates. An eight-noded and a sixteen-noded solid-like shell element are derived. The sixteen-noded solid-like shell element is displayed in Figure 2. In addition to the geometrical nodes 1-16, four internal nodes are defined in the middle of the four corners of the element. Through the location of the nodes an isoparametric frame of reference is spanned,

*e *

= (~, 11, ### Sl .

In the undeformed state each material point X in the element can be written as a function of the isoparametric coordinates(~m' 11m' Sm) :

(1)

In eq.(l) the vector

### X"

represents the projection of the material point onto the mid-surface of the element. The vector D represents the thickness director in this point, see Figure 3. The position x of*the same material point in the deformed configuration equals: x*= X +

*U,*in which the displacement field

*U*reads:

10

• geomeUicalnode

ill internal node

top surface mid-surface

bottom surface

*Fig. 2. Geometry of the sixteen-noded solid-like shell element. *

*Fig. 3. Kinematics of the sixteen-noded solid like shell element. *

The component *UO *denotes the deformation of the projection onto the mid-surface, the component u1

represents the deformation of the thickness director and

*w *

stands for the internal stretching which
is colinear to the thickness director *d*= D

### +

u1_{of the deformed configuration, Applying this }

formulation a linear strain in the thickness direction is assured, As a result, so-called "Poisson-Thickness-Locking" [3] is avoided, Based on the position vectors

*x *

and X the metric matrices gij and
Gij can be derived for the deformed and the undeformed configuration, respectively, Subsequently,

the components of the Green's strain tensor in a local frame of reference Ii are set up according to:

The local frame of reference is determined by the orientation of a characteristic material axis (e,g,
fibre orientation) and the shell thickness director D which leads to the factors t~ in eq,(3), After
some algebra the Green's strain tensor can be written as a function of the displacement field *u, *

When the interpolation of the displacement field is introduced, the components of the Green's strain tensor can be rewritten as a function of the nodal displacements,

(3)

To derive the stiffness matrix of the element the equilibrium in the weak form is established, After
some algebra the stiffness matrix *K *of the solid-like shell element and the internal force vector can
be derived, For a detailed description the reader is referred to [4, 12],

*2.2 * *Interface element *

To describe physically nonlinear effects like cracking and delamination interface elements have
been applied, Interface elements are elements of zero thickness which are inserted into the finite
element mesh at locations where cracking or delamination are expected to occur. In Figure 4
interface elements are displayed that can be combined with the sixteen-noded solid-like shell
element, and in particular the twelve-noded interface element is displayed in Figure 5, The
constitu-tive relation of interface elements is set up between the relaconstitu-tive displacements *v of the two adjacent *

layers of the interface elements and the tractions t in the interface. The relative displacement between the adjacent layers in a material point of the interface element can be written as:

(4)

### 16-noded solid-like shell

### s

### 7

### 12-noded interface element

*Fig. 5. Geometry of the twelve-naded intelface element. *

In eq.(4) the matrix R denotes the rotation matrix from the global into the local frame of reference.
The latter is defined in every material point of the interface element by the two tangential directions
and the normal direction of the layer, Figure 5. The matrix *L *is a mapping matrix which maps the
*displacements of the adjacent layers onto their relative displacements. The matrix B contains the *
shape functions which are dependent on the isoparametric variables ~ and 17. The vector ug contains

the nodal displacements of the interface element. When the equilibrium is established in the weak form, the stiffness matrix K and the internal force vector

### .tn

of the interface element can be derived:*K *=

*f f *

*B!DBg*

### detJod~d17

and:*fin*=

*f f *

### B~t

det### Jod~d17

(5)### s

'1### s

**11**

In eq.(5) the matrix D represents the material stiffness matrix and

*J" *

the Jacobian. In the elastic
regime the interface element represents a perfect bond between the adjacent layers. This is achieved
by using a high dummy stiffness.
### 3

### Residual strength analysis of centre cracked plates made of GLARE

*3.1 * *Interface crack model *

The use of interface elements to describe cracking introduces new degrees of freedom. Cracking occurs when a critical parameter, e.g. often the principal normal stress or critical K-factors, exceeds a certain threshold value. Then, a new degree of freedom is created at this node yielding a geo-metrical discontinuity. With interface elements cracking can occur between elements only and is therefore dependent on the original orientation of the finite elements. Since the direction of the crack growth is known due to experimental observations the discrete crack model combined with interface elements is a good approach to evaluate crack propagation [9, 14].

In interface elements the constitutive relation is set up between the relative displacements and the tractions in the interface. For the formulation of constitutive relation which governs the material behaviour and the description of the physically nonlinear effects different approaches are described

in the literature. Depending on the failure mechanisms for which the interface elements are applied the mathematical formulation can be based on an explicit traction! displacement relation [13], on a phenomenological plasticity approach [15] or on a damage theory [1].

When cracking is described with interface elements the assumption of a perfect bond between the two adjacent layers must be modified. In a general situation all three traction components in the plane of cracking contribute to the initiation of a crack. For a fully open crack this means that no stress can be transferred in any of the three directions in the plane of cracking, even under single-mode loading. To account for this effect a loading functionfis now introduced. This loading function bounds all states of traction in the interface. Inelastic deformations occur when a state of traction violates the loading function. For the present model these inelastic deformations represent the crack opening in a material point. In the limiting state of a fully open crack the loading function shrinks to a point in the origin of the traction space. This implies that no load can be transferred in the material point, not even in compression. The loading function

*f *

reads:
~.

*j(t, *7C) = ~2t Pt-t(7C):SO; _{P }=

### [

### ~

### ~

0 2 0### oj

002

(6)

with:

In eq.(6), the quantity

*t *

denotes the equivalent traction and the matrix P is set up with reference to
von Mises plasticity. The shape of the loading function is given in Figure 6. When a state of traction
violates the loading function a return-mapping algorithm must be applied which maps the state of
traction back onto the surface of the loading function while the inelastic deformations grow. Then,
the relative displacement increment is decomposed into an elastic part and an inelastic part, which
gives:
(7)

Applying an associative flow rule the incremental crack opening deformations *vee can be written as: *
(8)

In eq.(8) LI..?c represents the finite amount of inelasticity and the gradient

*(df! *

*at)*sets the direction of the crack opening deformations. The increment of the elastic relative displacements Ll.ve1 is related to the traction increment Ll.tn+! at the end of the loading step via the linear elastic stiffness matrix D:

Upon substitution of eq.(7) and eq.(8) into eq.(9) we obtain the traction increment which finally leads to the tractions:

with:

(9)

If the trial traction tt"ol violates the loading function, eq.(6), the corresponding tractions and the

crack opening deformations are calculated according to:

and: (11)

The latter two equations represent a system of four equations with five unknowns: t, *K, LlA . *For the
final solution of eq.(ll) a hardening hypothesis must be introduced which sets the relation between

LlAn+l and LlKn+l' Applying eq.(ll) and the hardening hypothesis *LlK *= *f(LlA) *the loading
function *f *can be rewritten as a function of *LlK *only [5]. Starting with *LlKO *= 0 a new *LlK *can be
calculated applying a Newton-Raphson procedure which reads:

k + 1 _ k

*f *

### I"

*LlKn+1 -* LlKn + 1 - *dfldLlK *
n+1

(12)

Subsequently, the new *LlA *and new tractions t are computed [5].

*Fig. *6. *Surface of the loading function applied with interface elements to describe cracking. *

*Fig. *7. *Equivalent stress as junction of the softening parameter K. *

*3.2 * *Hardening hypothesis *

For the derivation of the return-mapping algorithm, a modified work hardening hypothesis is applied which reads in an incremental manner:

(13)

The computed *J(= *1'iJ + L\.J(can directly be compared with the fracture toughness G, of the material.

*3.3 * *Function of the equiva lent traction *

Similar to the traction-separation law by Tvergaard and Hutchinson [17] the function *t( J() *is a
phe-nomenological representation of the fracture process and not a description of the atomic separation.
In the present model the fracture process is initialised when the yield stress

*ay *

is reached. Upon
fur-ther loading the stress increases from the yield stress *ay*up to the ultimate stress au of the material, Figure 7. When the ultimate stress is reached the plastic work per unit surface area equals the criti-cal fracture toughness Gc of the material. At this point the crack is fully opened and the dissipated energy equals the fracture energy. The stress has been reduced to zero while the inelastic relative displacements continue to grow. To obtain a smooth transition from the hardening to the softening branch, the hardening regime is described by a quadratic function:

(14)

and the softening regime is described by an exponential function:

with:

*k *

= ### {(iG~cy

(15)The parameter

*f3 *

determines the rate of softening. For a sharp decrease *f3 *

= 0.5 is chosen.
*The hardening and softening branch are shown schematically in Figure 7. The residual stress o;ee is a *
*small value (a"e *= *10-2 _{MPa) }*

_{in order to achieve numerical stability for the return-mapping }algorithm. Next to the return-mapping algorithm the consistent tangent stiffness matrix is applied to assure efficient and stable numerical simulations [5].

*3.4 * *Centre cracked plate made of GLARE™ *

In the following the behaviour of a centre cracked plate made of GLARETM is studied. The width of
the plate equals 400 mm and its length is 800 mm. Due to geometrical symmetry and material
sym-metry only one quarter of the plate is modelled with sixteen-noded solid-like shell elements. At the
symmetry line, starting from the crack tip onwards interface elements are located. Here, the
dis-placements in the iI-direction of one plane of the interface elements (in Figure 8 the right plane) are
restrained. In the i2-direction the displacements of both planes of the interface elements are equal.
Thus, pure mode-I cracking is enforced. The plate is loaded with a distributed load as depicted in
Figure 8. The material parameters for GLARETM and the interface crack model are given by Hashagen
et al. [7]. Plasticity in the plate is accounted for by an anisotropic plasticity model [8] which has been
applied with a yield stress aiieneiOn) = *320MPa *and a;ien'iOn) = *360MPa, *respectively.

In Figures 9 and 10 the crack length extension and the crack mouth opening displacement of the centre cracked plate are displayed. From these graphs we can conclude that the numerical results

obtained with the interface crack model agree well with the experimental results [18]. Depending on
the yield stress 0"11 the computed ultimate loading lies within a range of five percent of the
experimental value O"gW% = 319 *MPa. *

In Figure 11 the distribution of the normal traction is visualised for the interface elements which are located along the i2-axis of the model, see Figure 8. The load levels refer to the external loads (a)-(d) which are marked in Figure 9. We observe that the stress decreases sharply when the ultimate stress of the material is reached. The distribution of the dissipated energy is visualised in Figure 12. The location of the sharp growth of the dissipated energy again coincides with the location of the ultimate stress in the traction profile. This position indicates the location of the crack tip which is displayed in Figure 10. Due to the choice of the exponential softening function, in which the equivalent stress does not become zero, the traction in the interface remains at a small residual value in the fully cracked situation. Due to imperfections in the plate buckling is observed in most of the experiments. Here buckling is understood as a movement of material points out of the plane in which the plate is located. In the experiments buckling can prevented by so-called anti-buckling guides. To compare experimental and numerical results when anti-buckling guides are not mounted to the plate an imperfection is applied to the finite element model. For this purpose an out-of-plane force is imposed on the cracked plate prior to the inplane loading. The small force

P = *0.05N *which triggers buckling acts on the plate at the centre of the crack, point A in Figure 8.

In Figure 13 the crack length extension is visualised. Again, we observe that the calculated crack
length extension agrees well with the experimental values. Especially, the residual strength of the
plate matches with the experimental value. Also, the rate of crack growth calculated in the
numeri-cal analysis agrees with the experimental observations. In Figure 14 the gross stress is displayed as a
function of the out-of-plane displacement of point A. It can be observed that the load at the onset of
buckling calculated in the numerical analysis agrees with the experimental value. The dissipated
energy and the traction profile in the interface elements show the same characteristics as for the
plate without buckling. In Figure 15 the deformed state of the cracked plate is displayed for the load
levels O"gwe, = *250MPa *of the pre-peak regime and the post-peak regime, respectively. The
out-of-plane displacement is clearly visible and has a maximum value at the centre of the crack (point A).

*Fig. *8.
applied
gross
stress
O"gross
interface elements
rigid

### ~---==;;-:,-:-;:-==~,-;=-;-"." ~I

cral:k lcngth### I

0 extension da tr, : o __________ initial crack*-1, ____ *

*-"-3:c:c*

*S('-.)*- - - I .. ..j-I

### ~L~'

### pom',':"h '0

elongation du### ..

crack mouth opening displacement CMOD

II

*Geometrical properties (in *[111111]) *and boundary conditions of the centre cracked plate with a *
*thickness *1.4111111 *that is made ofGLARPM. *

Gross stress [MPa] 400

### ,.---r---,...----,

300 200 100 0 0*Fig.*9.

### -... cry'''d

### =

360 MPa### Mcr.

### =

320MPa 2 4 6Crack mouth opening displacement [mm]
*Gross stress versus crack mouth opening *
*displacement of the centre cracked plate *
*made ofGLARETM. *

Interface traction [MPa]

1200

### r---,r===:=.=:===i1

: 00 load level (a)

600

-300

i . . load level (b) - 00 load level (c)

liliiii load level (d)

100 Position [mm]

150

*Fig. *11. *Distribution of the normal traction in the *
*interface of the centre cracked plate *
*madc of GLARETM for different load *
*levels. *

Gross stress [MPa]

340 , - - - . . , - - - , - - - , 300 280 260 240 220 20 40

Crack length extension [mm]
*Fig. *10. *Gross stress versus the crack length *

*extension of a centre cracked plate *
*made of GLARETM . *
Dissipated energy [N/mm]
60
500

### 'Fil=ii:::::;:;:-:---'-r===:=:::::=:==;:=:::;,

300 200 100 100 Position [mm] 150*Fig. *12. *Distribution of the dissipated energy in *
*the interface of the centre cracked plate *
*made of GLARETM for different load *
*levels. *

Gross stress [MPa] 320

### r----r--,----,---...,.---,

300 280 260 240 220 200 180 I I I I I I ~~--r---r---I---I I I I I ----~-- --~---~---I _ " - - ... ~ I I I I I I I I ---1---1---- ---1---I I I I I I I ---r---r---r---I I I I I I I I ______ L ______ L ______ L ______ L _____ _ I ______ ~---00 Experiment: Ita O"y',ld

### =

360 MPa### ---i--- -.

0".### =

320 MPa 160### L_l...'

### _--t:~~~::::E=-.J

### o

10 20 30 40 50Crack length extension [mm]
*Fig. *13. *Gross stress versus crack length extension *

*of the centre cracked plate made of *
*GLARETM with an imperfection. *

0.0 0.001 0.005

Gross stress [MPa]

350 , . . - - - . . . , . - - - - , - - - , . . - - - , 300 250 200 150 100 00 Experiment 50 - O"yj,ld

### =

360 MPa - . 0".### =

320 MPa### O~--~--~~~==~

### o

5 10 15 20 Out-of-plane displacement [mm]*Fig.*14.

*Gross stress versus out-of-plane*

*displacement of the centre cracked plate *
*made of GLARPMwithanimperfection. *

0.012 0.023

Equivalent plastic strain [mm/mm]

*Fig. *15. *Deformed configuration and equivalent plastic strain of the GLARETM plate with imperfection for *
*a gross stress of *250 *MPa: left: pre-peak loading, right: post-peak loading. *

### 4

### Delamination analysis of spliced tension specimen made of GLARE™

*4.1*

*Introduction to the splicing concept*

As a benefit of the layered composition of fibre metal laminates the splicing technique can be applied to increase the width of the fibre metal laminate sheets. The width of the aluminium layers is limited due to production aspects. But two or more aluminium layers can be connected by bridging prepreg layers which reduces the weight of the constructions for which fibre metal laminates are applied. In Figure 16 the principle of the splicing technique is displayed. The gaps

between the aluminium layers are filled with resin to avoid moisture contact. In the remaining, the aluminium layer which forms the gap is denoted as broken, and the layers which remain intact at the gap are denoted as bridging layers. As a result of the gap in the broken aluminium layer the load must be transferred to the prep reg layer and the aluminium layer that bridge the gap. There-fore, the interface between the broken aluminium layer and the bridging prepreg layer is loaded considerably. For high load levels the bond between the aluminium and the prepreg layer can become too weak. In the limiting case the bond disappears totally, the aluminium layer and prepreg layer are separated and delamination occurs, see Figure 17. For the description of delamination in composites various models and different concepts are detailed in the literature [1, 2, 11, 16]. Ladeveze and Allix introduce a damage parameter which describes the degradation of the stiffness of the interface upon loading. Konig and Kruger compute the mixed mode energy release rates and compare it with a critical energy release rate. In the present study the phenomenological approach by Schellekens and de Borst [16] is followed.

*4.2 * *Numerical formulation of the delamination model *

Similar to the interface crack model a loading function bounds all states of traction in the material point. If a state of traction violates the loading function, delamination is initialised. Then, the state of traction is mapped back onto the loading surface while the inelastic deformations grow. The material parameters describing the loading function are the tension strength

*tt, *

the
compres-sion strength *t, *

and the two shear strengths of the interface *t'i . *

The growth of the delamination is
described with the fracture toughness Gc In the limiting case when the energy dissipated by the
inelastic deformations equals the fracture toughness of the material a fully delaminated area has
occurred in the material point. The loading function *hd *

for delamination in the interface is displayed
in Figure 18 and reads:
with:

and:

*a = *1,2.

*Fig. *16. *Schematic sketch of a splice. *

prepreg layer prcpreg layer

(16)

(17)

loading direction

delamination

*Fig. *17. *Delamination of a spliced specimen. *

Loading function f

### I

K = 0.0### I

Loading function f I K = 1.0 Idirection Flow function g

*Fig. *18. *Loading function and plastic potential of the delamination model. *

In the limiting state when a material point has delaminated totally, shear tractions calmot be trans-ferred anymore. Therefore also the shear strengths

*fa *

depend on the softening parameter 1(. Since
the compressive strength is not affected by softening, for total delamination all states of traction are
*located on a straight line between the compressive strength and zero. The function s( K) is linear with *
8(0)

### =

1 and s(Gcl### =

O.If a state of traction violates the loading function (i.d < 0) a local return-mapping algorithm is carried
out. As a result the state of traction is mapped back onto the loading surface and the inelastic
defor-mations grow. Similar to the interface crack model the relative displacements are decomposed into
an elastic part 6.*vei *and an inelastic part 6.vid •

Here a non-associative flow rule is applied to avoid numerical problems [6]. The plastic potential from which the flow direction is derived consists of two regimes for positive and negative tensile

tractions, respectively. They differ in the set-up of the mapping matrix

### Pid.

Thus, the inelastic rela-tive displacement equals:; with (19)

and

d. [ 2 2 2 ]

lag

### (itS)2'(tdS)2'(i~2d

for a positive normal traction; (20)### Pid

diag[ 2 2 2 ]= etc)2' ctsld'

### (i~2d

for a negative normal traction. (21) When the modified work hardening hypothesis eq.(13) is applied the return-mapping algorithm and the tangent stiffness matrix can be derived. These algorithms are similar to those of the crack model. They are elaborated and described in detail by Hashagen et al. [6].*4.3 * *Delamination in spliced tension specimen *

To assess the behaviour of fibre metal laminates in the presence of splices two different configura-tions of spliced specimen are considered. The first configuration is composed of three aluminium layers and two prepreg layers. In this configuration two splices are located in the two outer alumin-ium layers. It is referred to as doubly spliced. The geometry and the boundary conditions of the finite element model for this design are displayed in Figure 19. The second configuration is referred to as asymmetrically spliced and consists of two aluminium layers with only one prepreg layer. Here, the splice is located in one of the outer aluminium layers. The geometry and the boundary conditions for this specimen are also displayed in Figure 19. The thickness of the aluminium layer equals

*t *

= 0.5 mm and the thickness of the prepreg layer is 0.125 mm. By virtue of symmetry only
one quarter of every configuration needs to be modelled with solid-like shell elements. Moreover,
the mid-surface of the doubly spliced specimen can be used as symmetry plane for a further
reduction of the finite element model. In the experiments a reference length of 50 mm is used to
calculate the strain. The splice is located in the middle of this reference length, see Figure 19.
Interface
clcments
doubly spliced
**strain **
rigid
loading
direction
Interface
e1cments
asymmetrically spliced
rigid
+---<0>-x

*Fig. *19. *Geometry and boundary conditions of the doubly spliced specimen (left) and the asymmetrically *
*splice specimen (right). *

The material data for the aluminium, the prepreg and the interface are given by Hashagell et al. [6].
Hereby, the fracture toughness of the material has been determined by various experiments
(de Vries et al.[19]). In the present study a fracture toughness Gc = 1.1 *N fmm *is used.
In the following, specimens are analysed in which the fibres in the prepreg are oriented in the
loading direction. The applied load is represented by the gross stress CJgm" which is the total load
divided by the unspliced cross area (12.5 mm x Itot"l) of the specimen. The components of the traction
are referred to the *X-, y-*and z-direction of the global frame of reference, Figure 19. The dissipated

energy can be decomposed into three components which also refer to the *X-, y-*and z-direction of the

global frame of reference.

In Figure 20 the stress-strain curve is displayed for the doubly spliced specimen with talu = 0.5 mm
and fibres oriented in the loading direction. The gross stress is also plotted versus the delamination
length, Figure 21. In the numerical model the delamination is initialised when the state of traction
first violates the loading functionJjd' Then, the delamination process starts and energy dissipates.
However, not all energy is dissipated at once. Therefore, material points in the specimen appear for
which delamination has just started and others which are fully delaminated. To assess the impact of
this process on the delamination length three different curves are plotted in Figure 21. The first
*curve is obtained for the position where delamination is initialised (K= 0.0 N fmm). *The second
*curve marks the position where fifty percent of the fracture toughness is dissipated (K= O.5Gcl and *
the third curve marks the position of the fully delaminated material points. It can be concluded that
the strain and the delamination length calculated numerically show a good agreement with the
experimental results, although the numerical analysis gives a slightly higher ultimate load.

Gross stress [MPa]

300

200

100 <II experiment 1, 2, 3

M numerical result ..., experimental ultimate load

0.5 1.0 Strain [%]

1.5

*Fig. 20. * *Gross slress versus slrain for the *
*doubly spliced specimen. *

2.0

Gross stress [MPa]

300 r----r----,---~----,---~ 200 100 ~ experiment 1, 2, 3 M numerical: K=O.O*G, .... numerical: K=0.5*G, W numerical: K=1.0*G. OL---~~==~==~~~

### o

*Fig.*21. 5 10 15 20 25 Delamination length [mm]

*Gross stress versus delamination*

*length for the doubly spliced specimen.*

In Figures 22-24 the normal traction and the two shear tractions, *t" * I, and

*ty *

are visualised for the
load levels (a)-(d) which are marked in Figure 20. We observe that the peak of the traction
components propagates in the x-direction when the load and subsequently the delamination length
increase. In the region which has been passed by the delamination front the tractions decrease again
to a near zero state. The shear traction component *ty*which is oriented perpendicular to the loading direction increases significantly at the free edge of the specimen in the region where delamination is

initialised. This behaviour can be explained by considering the djfferent lateral contractions of the layers which are loaded and which are unloaded when the delamination front propagates through the material. Due to the difference of the lateral contraction a relative displacement between the layers which bridge the splice and the broken layer is initialised. Consequently, a shear traction perpendicular to the loading direction is observed.

0.0

### -4.4

### -2.5

### -0.7

### 1.2

3.0*Fig. *22. *Traction profile in the z-direction in the inte!face of the doubly spliced specimen. *

*Fig. *23. *Traction profile in the x-direction in the intelface of the doubly spliced specimen. *

( c )
101m] _{20.0 }x _{0.0 } [mm]
[MPa]
x

### x

20.0 1.7### 0.7

3.0 5.4### 7.8 [MPa]

*Fig. *24. *Traction profile in the y-direction in the interface of the doubly spliced specimen. *

The dominant role of the shear component in the loading direction is also emphasised when the dissipated energy is studied. In Figures 25 - 27 the energy is displayed which is dissipated in the normal direction and the two shear directions, Z-, y-and x-direction, respectively. In Figure 26 we

observe that the energy dissipated in the z-direction of the model (normal direction of the interface) is less than the energy dissipated in the x-and y-directions which form the two shear components of the interface. Furthermore, the zone where energy is dissipated in the z-direction is restricted to the tip of the splice and does not grow in the x-direction when the specimen is loaded, see Figure 26. In contrast to this observation we can see that the zone where energy is dissipated in the x-direction and in the y-direction grows when loading the specimen. In particular, the energy which is dissipated in the x-direction of the specimen is much larger than the energy dissipated in the y-direction. In the centre of the specimen the x-component of the dissipated energy reaches nearly the fracture toughness of the interface. However, at the free edge of the specimen a significant y-contribution to the dissipated energy can be noticed. Similar to the traction component, the differ-ences in the lateral contraction between the bridging layers and the broken layer are responsible for the energy dissipation in the y-direction. When delamination occurs the bridging layers are loaded further while the broken layer unloads. This induced difference in the displacement of the layers results in a considerable energy dissipation.

0.0 0.25 0.5 0.75

### x

20J)

LOS [NfmmJ

*Fig. *25. *Dissipated energy in the x-direction in the interface of the doubly spliced specimen. *

y ( a ) ( d ) 6.25 f···,··· ... , 6.25 fr.···,···,··· ...•...•...•... , 0.0 I"-'----'----~----~---'-i ... 0.0 0.0

### Imml

20.0### x

0.0 I. 0.0 1.7 3.4### ImmJ

5.1 .7 x 20.0 6.8 [10·*N/mm]*

0.0 0.04 0.08 0.12 0.16 [N/mmJ

*Fig. *27. *Dissipated energy in the y-direction in the interface of the doubly spliced specimen. *

*4.4 * *Asymmetrically spliced specimen *

The asymmetrically spliced specimen is analysed in the same manner as the doubly spliced
specimen, but now the aluminium layer is 0.3 mm thick. For the asymmetrically spliced specimen
the assumption of a geometrically linear behaviour has a strong impact on the results and leads to a
significant difference between numerical and experimental data. In Figures 28 and 29 the
displace-ment of the tip of the splice in the z-direction is displayed versus the applied load. The two graphs
are obtained assuming a geometrically linear formulation and a geometrically nonlinear
formula-tion respectively. Obviously, the displacement in the z-direcformula-tion grows steadily when a
geo-metrically linear behaviour is assumed. In contrast, for the geogeo-metrically nonlinear formulation the
displacement in the z-direction passes a maximum and decreases slightly afterwards. In the present
calculation the maximum displacement is approximately 0.12 mm. The out-of-plane displacement
in the z-direction can be explained with the location of the neutral axis of the specimen. Except for
the region around the splice, the neutral axis of the specimen is located in the middle of the prepreg
layer which is also, for this region, the symmetry line of the specimen. At the splice, however, one of
the two aluminium layers is broken and the lay-up is not symmetric anymore with respect to the
original neutral axis. Thus, at *the splice the neutral axis of the specimen is located in the bridging *

aluminium layer. When the specimen is loaded the difference of the positions of the neutral axis gives the maximum displacement of the bridging section in the z-direction. For the given geometry the maximum displacement is not higher than

*u, *

= 0.15 mm. In Figure 30 the gross stress is
dis-played versus the strain and in Figure 31 versus the delamination length for geometrically
nonlin-ear and geometrically linnonlin-ear formulation of the applied finite elements. Here, the differences
between geometrically linear and geometrically nonlinear formulation lead to a significant
differ-ence in the numerically calculated delamination length. For the geometrically linear formulation a
larger delamination length is computed. This length differs from the experimentally measured
delamination length. The latter matches with the numerically calculated delamination length when
a geometrically nonlinear behaviour is assumed. The formulation of the finite elements, either
geometrically linear or geometrically nonlinear, has a serious impact on the delamination process
computed in the numerical analysis. In Figure 32 the energy is displayed which is dissipated in the
z-direction of the specimen (mode-I). Again, the geometrically linear and nonlinear cases are
considered. The load levels (a) and (b) refer to a gross stress Cigw" = 250 MFa and Cigw,,= 340 MFa,
respectively, see Figure 30. Two major differences are noticed when the results obtained with the
two formulations *are *analysed. First, the total energy which is dissipated in the z-direction is more

than four times higher for the geometrically linear formulation compared with that of the geo-metrically nonlinear formulation. Secondly, the zone where energy is disSipated in the z-direction is larger for the geometrically linear formulation than for the geometrically nonlinear formulation. In Figure 33 the energy which is dissipated in the x-direction (mode-II) is visualised for the geo-metrically linear and for the geogeo-metrically nonlinear formulation. Again, the load levels (a) and (b) refer to the external forces (}gw",

### =

250 MPa and*(}gwo,*

### =

340 MPa, see Figure 30. We observe that thedissipated energy is larger for the geometrically linear formulation than for the geometrically non-linear formulation. Furthermore, the maximum of the dissipated energy in x-direction is not located at the tip of the splice as for the geometrically nonlinear formulation. Finally, at the free edge of the specimen less energy is dissipated in the x-direction for the geometrically linear formulation com-pared with the centre of the specimen.

z-displacement [mm] 50.0 40.0 30.0 20.0 10.0 100 200 300

Gross stress [MPa]
*Fig. *28. *Displacement in the z-direction of *

*the tip of the splice for geometrically *
*linear behaviour. *

Gross stress [MPa]

400 400 , - - - - , - - - - , - - - - r - - - - , 300 200 100 1.0 2.0 Strain [%] 3.0

*Fig. 30. * *Gross stress versus strain of the *
*asymmetrically spliced specimen *
*with t"H *= *0.3 mm. *
4.0
z-displacement [mm]
0.15
0.10
0.05
0.00 ' - - - ' - - - ' - - - - ' - - - '

### o

100 200 300 400*Fig.*29.

Gross stress [MPa]

*Displacement in the z-direction of the *
*tip of the splice for geometrically *
*nonlinear behaviour. *

Gross stress [MPa]

400 , - - - , - - - , 300 200 100 I I I I I ---~---~---An!. geom.lin., K=0.9*G, 00 geom.lin.,K=O.O*G, --- .. --- .... geom.nlin.,K=0.9*G, DO geom.nlin., K=O.O*G, . . experiment 1,2,3 0L---.b~=====~.d.J 0.0 10.0 Delamination length [mm] 20.0

*Fig. *31. *Gross stress versus delamination length *
*of the asymmetrically spliced specimen *
*with t"H *= *0.3 mm. *

[N/mml IN/mm]

[N/mm] [N/mmJ

*Fig. *32. *Dissipated energy in the z-direction in the inteJface of the asymmetrically spliced specimen. *

[N/mml IN/mm] 6.25

### I

0.0 20.0 0.0 fN/mm] IN/mm]### 5

### Conclusions

In the present paper a numerical strategy has been introduced to describe crack propagation and delamination propagation in fibre metal laminates. The strategy has been based on a solid-like shell element and corresponding interface elements. The interface elements have been located in the finite element mesh at positions where either cracking or delamination is expected to occur. Crack-ing and delamination have been accounted for by the introduction of loadCrack-ing functions which bound all states of traction in the interface. When a state of traction violates the loading function a return-mapping algorithm is carried out to map the state of traction back onto the surface of the loading function. Due to this process energy is dissipated. When the dissipated energy equals the fracture toughness a fully cracked or fully delaminated area occurs.

The numerical models have been applied successfully to a residual strength analysis of centre cracked plates made of GLARETM. Here, the numerical results show a good agreement with the experimental data. Especially, the residual strength of the plate and the rate of crack growth has been represented correctly. Furthermore, the calculated out-of-plane displacement of a centre cracked plate with imperfection agrees with the experimental observations. The material data which serve as input for the numerical model have been derived from theories that are applied for homogeneous material. Thus, the good agreement between experimental and numerical results justifies the application of these theories for fibre metal laminates.

Finally, delamination in spliced tension specimen made of GLARETM has been studied. Here, it has been found that mode-II delamination plays a dominant role in the delamination process. A note-worthy contribution of mode-I delamination occurs only at the tip of the splice and only for the initialisation of delamination. It appeared that geometrically nonlinear behaviour must be taken into consideration for the asymmetrically spliced tension specimen. For the delamination analysis too, the numerical models have led to a better understanding of the delamination process in fibre metal laminates.

### References

[1] ALLIX O. and LADEVEZE P., Modelling and computation of delamination for composite
*lami-nates, Arch. Mech., 44, 5-13 (1992) *

[2] CORIGLIANO A., Formulation, identification and use of interface models in numerical analysis of
*composite delamination, Int. *

### J.

*Sol. Struct.,*30(20), 2779-2811 (1993)

[3] BISCHOFF M. and RAMM E., Shear deformable shell elements for large strains and rotations,
*Int. *

### J.

*Numer. Meth. Engng.,*40, 4427-4449 (1997)

[4] HASHAGEN F., A geometrically and physically nonlinear layered solid-like shell element,
*TU Delft report I1r.: 03-21-0-31-22, *Delft University of Technology, Delft, The Netherlands,
(1995)

[5] HASHAGEN F., An interface element for crack modelling in aluminium, *TU Delft report I1r. *
*03-21-0-31-22, *Delft University of Technology, Delft, The Netherlands (1996)

[6] HASHAGEN F., BORST R. DE and VRIES T. DE, Delamination behaviour of spliced fibre metal
*laminates, part II: numerical investigation, Int. *

### J.

*Compo Struct.,*(submitted for publication)

[7] HASHAGEN F., BORST R DE, Modelling onset and growth of mixed-mode cracking in fibre metal
*laminates, Proc. *4'" *World Congo Camp. Mech., *(to appear)

[8] HASHAGEN F., BORST R DE, A plasticity model including anisotropic hardening and softening for
*composite materials, in: Finite Elements in Engrg. and Scien. Proc. *2Hd *Int. DIANA Can! *eds.:

HENDRIKS M.AN., JONGEDl)K H., ROTS J.G., VAN SPANJE W.J.E. and BLAKMA, AA Rotterdam, The Netherlands, pp. 1139-1147 (1997)

*[9] HOHBERG J.-M., A joint element for the nonlinear dynamic analysis of arch dams, Dissertation, *
ETH Zurich, Zurich, Switzerland (1992)

[10] HORST P. and OHRLOFF N., Possible application of GLARE material as shown by the example of
*the AIRBUS A330, Proc. Deutsch. Luft- und Raumfahrt/congrefl1994 - DGLR-Jahrestagung, ed.: *
Burgener G., Erlangen, Germany, 591-600, (1994)

[11] KONIG M. and KRUGER R, Computation of energy release rates: a tool for predicting
*delami-nation growth in carbon fibre reinforced epoxy laminates, Proc. 4th Int. Con! Compu. Plast. *

*COMPLAS IV, *eds. OWEN D.RJ., HINTON E. and ONATE E., Pineridge Press, Swansea, U.K.,

1167-1178 (1995)

*[12] PARISCH H., A continuum-based shell theory for non-linear applications, Int. *

### J.

*Num. Meth.*

*Engrg.,*38 (11),1855-1833 (1995)

[13] *ROTS J.G., Computational modeling of concrete fracture, Dissertation, Delft University of *
Technology, Delft, The Netherlands (1988)

[14] ROTS J.G. and SCHELLEKENS

### J.CJ.,

*Interface elements in concrete mechanics, in: Computer Aided*

*Analysis and Design of Concrete Structures,*eds.: Bicanic N., Mang H., Pineridge Press, Swansea, Wales, UK, 909-918 (1990)

[15] SCHELLEKENS

### J.CJ.,

*Computational strategies for composite structures, Dissertation, Delft*University of Technology, Delft, The Netherlands (1992)

[16] SCHELLEKENS

### J.CJ.,

and BORST R DE, Free edge delamination in carbon-epoxy laminates: a novel*numerical/ experimental approach, Compo-. Struct., 28, 357-373 (1994)*

[17] TVERGAARD V. and HUTCHINSON J.W., The influence of plasticity on mixed mode interface
*toughness,]. Mech. Phys. Solids, 41(6),1119-1135 (1993) *

[18] VRIES T. DE, Various parameters concerning the residual strength of aircraft materials, part II:
*test data and charts, Graduation thesis, Delft University of Technology (1994) *

[19] VRIES T. DE, VWT A, HASHAGEN F., Delamination behaviour of spliced fibre metal laminates,
part I: *experimental results, Int. ]. Compo Struct., (submitted *for publication)